- Home
- Documents
*DETERMINATION OF DENSITY AND MOISTURE CONTENT OF … · DETERMINATION OF DENSITY AND MOISTURE...*

Click here to load reader

View

16Download

0

Embed Size (px)

DETERMINATION OF DENSITY AND MOISTURE CONTENT OF WOOD USING TERAHERTZ TIME DOMAIN SPECTROSCOPY

by

Belal Ahmed

B.Sc., University of Ain-Shams, 2007

THESIS SUBMITTED IN PARTIAL FULFILLMENT OF THE REQUIREMENTS FOR THE DEGREE OF

MASTER OF SCIENCE IN

PHYSICS

UNIVERSITY OF NORTHERN BRITISH COLUMBIA

October 2014

© Belal Ahmed, 2014

UMI Number: 1526479

All rights reserved

INFORMATION TO ALL USERS The quality of this reproduction is dependent upon the quality of the copy submitted.

In the unlikely event that the author did not send a complete manuscript and there are missing pages, these will be noted. Also, if material had to be removed,

a note will indicate the deletion.

Di!ss0?t&iori P iiblist’Mlg

UMI 1526479Published by ProQuest LLC 2015. Copyright in the Dissertation held by the Author.

Microform Edition © ProQuest LLC.All rights reserved. This work is protected against

unauthorized copying under Title 17, United States Code.

ProQuest LLC 789 East Eisenhower Parkway

P.O. Box 1346 Ann Arbor, Ml 48106-1346

Abstract

Terahertz time-domain spectroscopy was used to simultaneously predict the density and

moisture content of four wood species (Aspen, Birch, Hemlock and Fir). Using a fixed value for the

dielectric function of water, it was found that moisture content was systematically underestimated at low

moisture contents, which results from changes in the dielectric function of water as it goes from free to

bound in nature. The variation of the dielectric function of water with moisture content was studied

further, and the results show that the dielectric function of water does indeed change with moisture

content. The results are a large step forward in our understanding of wood-water interactions at Terahertz

frequencies, and therefore useful for applications in wood science.

List of papers

This thesis is the outcome of my M.Sc. studies in the Department of Physics at the

University of Northern British Columbia, Prince George, BC, Canada, from September 2012 to

August 2014. The work has resulted in two papers and one invited conference presentation as

listed below.

Paper I / Chapter 3 T. Inagaki, B. Ahmed, I. D. Hartley, S. Tsuchikawa, and M. Reid, " Simultaneous prediction of density and moisture content of wood by terahertz time domain spectroscopy", J Infrared, Millimeter, and Terahertz Waves. (2014) 35:949-961

Paper II / Chapter 4 B. Ahmed, I.D. Hartley, E. Jensen, T. Inagaki, S. Tsuchikawa, and M. Reid “Investigation of the water absorption in wood by terahertz time-domain spectroscopy”, To be submitted to the Journal of Infrared, Millimeter, and Terahertz Waves.

Conference: M. Reid, T. Inagaki, I. D. Hartley, B. Ahmed, K. Lawyer, S. Tsuchikawa, and A. Nasr, “Terahertz spectroscopy of wood and combustion gas”, CAP Congress, 2014, Ontario, Canada. [71].

Contributions

Paper I: I took an active part in sample preparation, data analysis and writing of the manuscript.

Paper II: I developed the model, performed simulation work, data analysis, and wrote the manuscript.

Table of Contents

Abstract..............................................................................................................................................i

List of papers ......................................................................................................................................ii

Table of contents............................................................................................................................. iii

List of figures................................................................................................................................... v

Acknowledgments........................................................................................................................... ix

1. Introduction ................................................................................................................................1

2. Background................................................................................................................................ 5

2.1 THz spectrum.................................................................................................................... 5

2.2 Terahertz time-domain spectroscopy (THz-TDS) ..............................................................6

2.3 Terahertz emission...............................................................................................................9

2.4 Terahertz detection............................................................................................................ 12

2.5 Effective medium theory................................................................................................... 14

2.6 Wood structure.................................................................................................................16

2.6.1 Softwoods and hardwood.....................................................................................17

2.7 Moisture content..............................................................................................................21

2.8 Density.............................................................................................................................22

2.9 Applications of THz technology......................................................................................23

2.9.1 Using terahertz radiation to probe wood..............................................................25

2.9.2 Analysis of THz data ............................................................................................26

2.9.3 The inverse electromagnetic problem..................................................................28

3. Simultaneous prediction of density and moisture content of wood by terahertz time

domain spectroscopy

3.1 Abstract............................................................................................................................. 32

3.2 Introduction.......................................................................................................................33

3.3 Materials and methods......................................................................................................35

3.3.1 Sample preparation...............................................................................................35

3.3.2 THz spectral measurement................................................................................... 37

3.4 Results and discussion...................................................................................................... 37

3.5 Conclusion........................................................................................................................54

4. Investigation of the water absorption in wood by terahertz time-domain spectroscopy

4.1 Abstract............................................................................................................................. 56

4.2 Introduction....................................................................................................................... 57

4.3 Materials and methods......................................................................................................60

4.3.1 Sample preparation............................................................................................... 60

4.3.2 THz spectral measurement................................................................................... 61

4.4 Results and discussion......................................................................................................62

4.5 Conclusion........................................................................................................................ 74

5. Conclusion................................................................................................................................ 76

IV

List of Figures

2.1 Electromagnetic Spectrum ....................................................................................................6

2.2 THz waveform with and without 1mm thick Aspen. The samples have dimensions of 30

mm x 30 mm at a moisture content of 28% ......................................................................7

2.3 Experimental arrangement for THz-TDS spectroscopy measurements. A THz pulse is

obtained when focusing the pump beam onto the photoconductive emitter. The probe

beam gates the photoconductive detector co-incident with the THz pulse. By changing the

optical delay between probe and THz pulses, the time evolution of the THz pulse is

obtained ............................................................................................................................... 9

2.4 Photoconductive THz transmitter. The pump beam illuminates the biased antenna with

photon energies greater than the band gap. THz radiation is then radiated from the

resulting transient photocurrent according to Maxwell's equations with wavelengths in the

terahertz range.....................................................................................................................11

2.5 Photoconductive THz receiver. The probe beam gates the photoconductive detector by

creating a transient conductivity window ..........................................................................13

2.6 Softwoods: internal structure .............................................................................................. 18

2.7 Hardwoods: internal structure ............................................................................................ 19

2.8 Softwood (left) and hardwood (middle, right) cell wall structure ..................................... 20

2.9 Free and bound water inside wood......................................................................................22

2.10 THz transmission spectroscopy...........................................................................................26

V

2.11 Fabry-Perot reflections....................................................................................................... 29

3.1 Dependence of moisture content (oven-dry basis) on the variation in relative humidity for

maple (open circle), aspen (filled circle), birch (open square) and Western hemlock (filled

square)................................................................................................................................ 38

3.2 Frequency-resolved (a) real part and (b) imaginary part of the dielectric function obtained

from THz transmission spectroscopy of oven-dry wood. Relation between oven-dry

density and (c) real part and (d) imaginary part of dielectric function averaged over the

frequency range of 0.1 to 0.2 THz (polarization of the THz field is perpendicular to the

grain of the wood samples) ................................................................................................39

3.3 Frequency-resolved (a) real part and (b) imaginary part of the dielectric function obtained

in transmission spectroscopy of Birch at various moisture content. Relation between

moisture content and (c) real part and (d) imaginary part of dielectric function averaged

over the frequency range of 0.1 to 0.2 THz (polarization of THz field is perpendicular to

grain of wood) ................................................................................................................... 40

3.4 Composite Cylinder Assemblage (CCA) scheme where a cylindrical inclusion of

dielectric constant ^ is surrounded by a cylindrical shell of dielectric constant e2 leading

to a bulk effective dielectric function £eff ......................................................................... 42

3.5 Effective medium theory applied to determine the bulk effective dielectric function of

wood at different moisture contents. The dry cell wall material with dielectric constant

£0Vencw (which is known from measurement - see text for details) is combined with a

random distribution of water assumed to have a dielectric function £water (see text f°r

details) using the Bruggeman model to determine the effective dielectric constant of the

wet cell wall material. The MG model with cylindrical symmetry is then applied to

combine air, with a dielectric function £air, and the wet cell wall material to determine the

effective dielectric constant of the wood, ewetwood .........................................................................46

3.6 Typical set of reference (dot line) and sample (solid line) waveforms along with the best-

fit predicted waveform (dashed line) according to the model .......................................... 50

VI

3.7 Relationship between measured and predicted density based on MG-EMT model, r 2,

determination coefficient; RMSE, root mean square error, (a) Perpendicular and (b)

parallel refer to the polarization of the THz field with respect to the grain of the wood

samples............................................................................................................................... 52

3.8 Relationship between measured and predicted moisture content based on MG-EMT

model, r 2, determination coefficient; RMSE, root mean square error. Perpendicular and

parallel refer to the polarization of the THz field with respect to the grain of the wood

samples............................................................................................................................... 53

4.1 Dependence of the THz field amplitude on the variation of MC in wood. These data are

taken at MC between 0% and 30% .................................................................................... 63

4.2 Real part of the dielectric function between 0.2 and 0.5 THz obtained from THz

transmission spectroscopy of 4 different wood species which are: (a) Birch, (b) Aspen, (c)

Hemlock, and (d) Fir, for the parallel orientation of the wood grain with respect to THz

field polarization at MC between 0% and 30% .................................................................64

4.3 Imaginary part of the dielectric function between 0.2 and 0.5 THz obtained from THz

transmission spectroscopy of 4 different wood species which are: (a) Birch, (b) Aspen, (c)

Hemlock, and (d) Fir, for the parallel orientation of the wood grain with respect to THz

field polarization at MC between 0% and 30% .................................................................65

4.4 Real part of the dielectric function of wood obtained from THz transmission spectroscopy

of 4 different wood species which are: (a) Birch, (b) Aspen, (c) Hemlock, and (d) Fir.

The polarization of the THz field is parallel to the wood grain, and the results are plotted

for a frequency of 0.3 THz ................................................................................................66

4.5 Imaginary part of the dielectric function of wood obtained from THz transmission

spectroscopy of 4 different wood species which are: (a) Birch, (b) Aspen, (c) Hemlock,

and (d) Fir. The polarization of the THz field is parallel to the wood grain, and the results

are plotted for a frequency of 0.3 T H z...............................................................................67

VII

4.6 The real part of the dielectric constant of water at MCs from 1% to 29% for the four

wood species: (a) Birch, (b) Aspen, (c) Hemlock, and (d) Fir. The upper thick line

represents the real part of the dielectric constant of free water and the lower thick line

represents the real part of the dielectric constant of ice as per references [68, 69]

respectively......................................................................................................................... 69

4.7 The imaginary part of the dielectric constant of water at MCs from 1% to 29% for the

four wood species: (a) Birch, (b) Aspen, (c) Hemlock, and (d) Fir. The upper thick line

represents the imaginary part of the dielectric constant of free water and the lower thick

line represents the imaginary part of the dielectric constant of ice as per [68, 69]

references respectively....................................................................................................... 70

4.8 Real part of the dielectric function of water obtained from THz transmission spectroscopy

of 4 different wood species which are: (a) Birch, (b) Aspen, (c) Hemlock, and (d) Fir.

The polarization of the THz field is parallel to the wood grain, and the results are plotted

for a frequency of 0.3 THz ................................................................................................ 73

4.9 Imaginary part of the dielectric function of water obtained from THz transmission

spectroscopy of 4 different wood species which are: (a) Birch, (b) Aspen, (c) Hemlock,

and (d) Fir. The polarization of the THz field is parallel to the wood grain, and the results

are plotted for a frequency of 0.3 TH z............................................................................... 74

VIII

Acknowledgments

"If the facts don’t fit the theory, change the facts" -Albert Einstein

I would like to express the deepest appreciation to my supervisors, Dr. Ian Hartley, and

Dr. Erik Jensen. Special thanks go to Dr. Matthew Reid, who has the attitude and the substance

of a genius. Without his guidance and persistent help this dissertation would not have been

possible. Furthermore, I would like to thank Dr. Tetsuya Inagaki for providing me with a lot of

important advice.

Above all, I am so grateful for being blessed with a wonderful child, Malak Ahmed, and a

wonderful wife Radwa Hammad. This thesis would not be possible without the love and support

of my mother, Eman Eltaweel, and my father, Mohamed Esawe. Not only have they encouraged

me throughout my studies, but provided me with the work ethic and motivation to succeed.

Finally, I am very thankful to everybody who was important to the successful completion

of this thesis.

IX

Chapter 1

Introduction

Terahertz (THz) radiation lies in the far infrared portion of the electromagnetic

spectrum. The possibility for sub-mm imaging capabilities together with the possibility for

collecting spectroscopic information, makes this part of the electromagnetic spectrum very

attractive for many applications and offers unique capabilities that can be applied to non

destructive testing of materials. The most useful frequency range for applications in wood

science fall below about 1 THz [1] with sub-millimeter spatial resolution that is not possible at

lower frequencies such as microwave frequencies. Most non-conductive dry materials are

transparent in the far infrared spectral region and many materials have ‘terahertz fingerprints’,

permitting them to be identified, analysed and imaged. The non-ionizing properties of terahertz

radiation and the extremely low power levels typically used make it a safe technology in

comparison to X-rays for example. Additionally, THz radiation is sensitive to the internal fibre

structure of wood and wood composites [2]. Transparency, good spatial resolution, safety of the

radiation and sensitivity to fiber structure make THz radiation an ideal technology to explore for

new applications in the wood products industry. In the past two decades, THz science and

1

technology has shown great potential, and many applications have been identified. THz radiation

shows a wide range of applications in the field of physical chemistry, spectroscopy of

pharmaceuticals and explosives [3], and medical technology [4], With respect to the wood

science field, THz radiation can be used to map density profiles of wood in transmission with

sub-annual ring resolution [5]. This transmission imaging is at exactly the spatial length scale

important for wood science, and subsequently has led to applications in dendrochronology [6].

There are different techniques that have been developed for studying the density of wood with

sub-annual ring resolution. These techniques are classified into, mechanical and spectroscopic

methods. The hardness feeler is one of the mechanical methods that was used to study the

density of wood, and uses a pin which is pressed into the wood at a defined pressure [7]. The

acid-corrosion method is one in which wood is burned by sulfuric acid and subsequently

scrutinized with an optical microscope [8]. In gravimetric-volumetric methods wood is cut into

slices and weighed and the volume is subsequently determined [9], Laser-sandblasting has been

used to study hardness profiles, and is implemented by sandblasting wood specimens [10]. The

common disadvantage of these mechanical methods is that they damage the sample under study,

and hence are destructive methods.

Many ranges of the electromagnetic spectrum have been used to study wood properties.

The electromagnetic spectrum is usually classified in terms of wavelength, frequency, or energy.

It includes radiowaves, microwaves, THz or far-infrared, infrared, visible light, ultraviolet, X-

rays, and y-rays in order of increasing frequency. Wood is opaque in the ultraviolet, visible and

infrared and imaging is therefore limited to reflection geometries [11]. In contrast, wood is

transparent at X-ray [12] and microwave [13] frequencies and measurements can be obtained in a

transmission geometry. Both microwave and X-ray methods are useful for defect scanning and

2

quality control and are currently used in the wood products industry. The ultimate spatial

resolution possible depends on the radiation wavelength, which means that sub-annual ring

resolution cannot be achieved with GHz frequency microwaves (~cm wavelengths). X-rays can

be used to get good spatial resolution; however, safety regulations need to be in place because

they are dangerous. For these reasons, it is useful to introduce new imaging techniques that have

good spatial resolution, are non-destructive, and safe to work with.

In this thesis, THz spectroscopy was used to perform transmission measurements in the

far-infrared range of the electromagnetic spectrum. The high sensitivity of THz radiation to

moisture content (MC) [14] offers the possibility for probing MC as well. Simultaneous

measurement of MC and density has only been demonstrated in a lab environment, using

microwave sensors. Although, there are limitations using these sensors such as the high noise in

amplitude and the restriction to one period for phase measurements [15], they remain important

to the wood products industry. It is therefore of interest to look at new techniques to

simultaneously measure MC and density; this problem is the subject of this thesis.

In order to simultaneously determine the wood density and MC, a number of systematic

studies were performed in this thesis. Before introducing these studies, background concepts are

presented in Chapter 2.

In Chapter 3, wood-water interactions are investigated using THz technology, which is

necessary to understand how moisture content affects the properties of wood at THz frequencies.

This is achieved by modeling the interaction of THz radiation with wood at different MC's and

comparing the model to experiments. In this experiment, four different wood species were

3

conditioned at different MC's. Density and MC effects of THz radiation interactions in wood

were studied using an effective medium theory (EMT).

In Chapter 4, the effect of MC on the dielectric function of water is studied to complete

the theoretical model developed in Ch.3. THz spectroscopy enables the investigation of water

dynamics due to its sensitivity to dielectric relaxation processes associated with water molecular

reorientation. The results show moisture content to be the major influencing factor for the

variation of dielectric properties of hydrated wood. As moisture content decreases, it is shown

that the dielectric function of wood decreases. A model for the dielectric function of water in

wood is developed, which allows us to study changes with moisture content as the water changes

from bound to free in form. This model for the dielectric function of water significantly advances

our understanding of THz-wood interactions.

4

Chapter 2

Background

2.1 THz Spectrum

The THz region of the electromagnetic spectrum lies in the far-infrared, between

microwave and infrared frequencies, (Figure 2.1). THz radiation is loosely defined by

frequencies between 0.1 and 10 THz. THz radiation has a submillimeter wavelength which

allows a good spatial resolution compared to microwave radiation. THz radiation is non-ionizing

and poses no significant health concerns [2] in contrast to X-rays. On the other hand, THz

radiation cannot penetrate metals and is strongly absorbed by water, being a polar molecular.

Most non-conductive dry materials are transparent at THz frequencies, which allow transmission

imaging. THz radiation is also sensitive to the internal fibre structure of wood and wood

composites which makes THz radiation of great importance to wood science [16].

5

Electromagnetic Spectrum

visible

106 107 10s lO10 1011 1012 1013 1014 1015 1016 1017 1018

Increasing frequency (Hz)

Fig. 2.1 Electromagnetic Spectrum.

2.2 Terahertz Time-Domain Spectroscopy (THz-TDS)

Terahertz transmission spectroscopy can be performed either directly in the time-

domain or in the frequency domain by Fourier transformation of the acquired data. The

measurement method used in this thesis is terahertz time-domain spectroscopy (THz-TDS)

where all the measurement are made in the time domain and the electric field is measured as a

function of time, which is possible because of the coherent detection using photoconductive

antennas.

In the time domain experiment, absorption results in a decrease of the amplitude and a

(possibly frequency-dependent) phase shift of the detected terahertz pulse. A temporal electric

field obtained from a THz-TDS spectrometer is shown in Fig. 2.2. The black signal represents

6

the reference signal where no sample is in place, and the red signal represents the signal that is

transmitted through the sample. By comparing the THz waveforms acquired with and without the

sample in place the complex permittivity and refractive index of the material under study can be

determined.

0.5ReferenceSample0 4 -

0.3

0.2

- 0.1

-0.2

- 0.3

- 0.42.2 2 3 2,4

x 10''°Time (s)

Fig. 2.2 THz waveform with and without 1mm thick Aspen. The samples have dimensions of

30 mm x 30 mm at a moisture content of 28%.

One of the original THz-TDS experiments was performed in 1989 by van Exter et al.

where the propagation of the terahertz pulses through water vapour was studied [19], While there

are many techniques to generate and detect THz radiation, the use of photoconductive antennas

7

that was reported in [19] was unique in that it employed coherent detection, mapping the THz

field directly in time. Most electromagnetic detectors measure the intensity of light and do not

resolve electromagnetic fields in time because of the extremely fast variation of the

electromagnetic field.

In order to achieve coherent detection, THz-TDS uses an ultrashort laser (on the order

of 100 femtosecond) to generate and detect the terahertz pulses. This ultrashort pulse is divided

into two parts, one part is used to generate the terahertz pulse and the other is to gate the detector

and arrives simultaneously with the terahertz pulse. Once the gate pulse arrives at the detector, a

current is generated that is proportional to the electric field of the terahertz pulse (which is the

coherent detection). Fig. 2.3 shows the experimental setup for THz-TDS spectroscopy, and the

physical mechanism behind generation and detection is discussed next.

8

Fig. 2.3 Experimental arrangement for THz-TDS spectroscopy measurements. A THz pulse is

obtained when focusing the pump beam onto the photoconductive emitter. The probe beam gates

the photoconductive detector co-incident with the THz pulse. By changing the optical delay

between probe and THz pulses, the time evolution of the THz pulse is obtained.

2.3 Terahertz emission

Generation and detection of pulsed THz radiation was first demonstrated using

photoconductive antennas by Auston et al. in 1984 [17]. There are many methods for generating

pulsed THz radiation, including nonlinear optical methods [18], and photoconductive antennas

[17, 18]. In this thesis, a photoconductive switch was used to generate and detect THz radiation,

and the principles of operation are described next.

9

Terahertz generation using photoconductive antennas

Figure 2.4 illustrates the mechanism of generation of THz radiation using a

photoconductive antenna. An ultrashort femtosecond laser (typically with a pulse width around

100 fs) illuminates a biased antenna on a semiconductor surface with photon energies greater

than the band gap, which creates a transient photocurrent. The transient photocurrent

]transient^) is generated by the acceleration of photocarriers in the bias electric field. Terahertz

radiation is then radiated from the transient photocurrent according to Maxwell's equations with

wavelengths in the terahertz range [18]. The THz radiated electric field, ETHz is directly

proportional to the temporal derivative of the transient photocurrent generated in the transmitting

antenna, A silicon lens is usually attached to the antenna to collimate the THz beam that is

generated as shown in Fig. 2.4.

1 0

Fig. 2.4 Photoconductive THz transmitter. The pump beam illuminates the biased

antenna with photon energies greater than the band gap. THz radiation is then radiated from the

resulting transient photocurrent according to Maxwell's equations with wavelengths in the

terahertz range.

THz radiation can be generated from a photoconductive antenna using a variety of

materials such as gallium arsenide (GaAs) and InGaAs, depending on the optical wavelength

used for excitation. Usually, a substrate with a short carrier lifetime in the sub-picosecond range

is desirable to maximize the variation of the transient photocurrent, which is why low

temperature (LT) GaAs, which has a sub-ps carrier lifetime, is often used instead of GaAs which

has a carrier lifetime with several hundred picoseconds [20], For this reason, low temperature

(LT) GaAs substrates are used in our system.

11

2.4 THz detection

There are two primary methods for the coherent detection of THz radiation: (1) electro

optic sampling and (2) photoconductive sampling. In this work, photoconductive sampling is the

method used for THz detection and details about this method and its advantages will be

discussed in the next section.

Terahertz detection using photoconductive sampling

THz detection using photoconductive sampling is similar to photoconductive generation

except that the bias electric field across the antenna comes from the electric field of the THz

pulse focused onto the antenna. A typical H-structured dipole photoconductive antenna is shown

in Fig. 2.4. An ultrashort femtosecond laser illuminates the 5 pm gap between the electrodes on

the semiconductor surface with photon energies greater than the band gap creating a transient

conductivity window. The THz field then drives a current proportional to the THz field over the

lifetime of the transient conductivity. This current is amplified and detected with a lock-in

amplifier at a frequency equal to the frequency at which the emitter bias is modulated. This

amplified current is then a convolution of the THz field and the transient photoconductivity

window. Because the window is short in time (sub-ps), the current collected is approximately

proportional to the THz field [29, 30],

X t ) = ^ f - E THz(t), Eq. 2.1

where ETHz{t) is the field of the incoming THz pulse, n(t), q, m are the density, charge, and

mass of the photocarriers respectively.

12

Electrodes

Fig. 2.5 Photoconductive THz receiver. The probe beam gates the photoconductive detector by

creating a transient conductivity window.

The antenna response function is frequency-dependent, and depends on the coupling of

the THz field into the antenna and the impendence matching conditions of the antenna to the

transmission line [21], In this work, TERA8-1 photoconductive antennas made from low

temperature (LT) GaAs substrates, were used to generate and detect THz radiation. These

antennas can generate THz radiation with a bandwidth up to about 4 THz. A Menlo system with

TERA8-1 photoconductive antennas was used to investigate the THz transmission through wood.

We also used a modified Picometrix T-Ray 4000 system (discussed later in the thesis), which is

also based on photoconductive emitters and detectors.

13

THz radiation is sensitive to water [32] which makes it a useful tool in predicting

moisture content (MC) in wood. The properties of wood (such as density and moisture content)

vary significantly within and between the different wood species, which affect structural

properties, and therefore dictate performance characteristics. In this work, a new THz-TDS

methodology to simultaneously predict density and MC is introduced. The ability to use THz

radiation to measure density and moisture content simultaneously is extremely important for the

wood products industry. In order to exploit THz technology for moisture content determination,

a model for the interaction with THz radiation is required. Wood contains 3 different materials:

air, water and cell wall material (cellulose, hemicellulose and lignin). Effective medium theories

(EMT) are traditionally used to look at composite systems, and were applied to wood in this

thesis to model the THz-wood interaction. The most commonly used EMT's are presented next,

and a basic overview of the characteristics of these models is introduced.

2.5 Effective Medium Theory

Maxwell-Garnett Model

The Maxwell-Garnet (MG) model is one of the most well-known EMTs and it is based

on analyzing the effective polarizability of spherical inclusions embedded in a host matrix. This

model is suitable to low volume fractions of inclusions. The MG model can be derived using

basic electrostatics and by knowing the permittivity of the host material [24], The expression

that gives the effective permittivity of the composite system is:

i«=£S. = / iElfS. Eq. 2.2£ R + 2 e h £p + 2 £ h

14

where £r is the effective permittivity of the composite medium; f^is the permittivity of the host

material; £p is the permittivity of inclusions; and f p is the volume fraction of inclusions. The

MG model is not generally used when a large contrast in permittivity between inclusions and

host exists [24], In such cases, other models are usually used to describe the permittivity of

composites. One such model is the Bruggeman model [25].

Bruggeman Model

The Bruggeman model in its basic form describes spherical particles embedded in a host

material, and can be used when a large contrast in permittivity exists. The basic form of the

Bruggeman model is given by Eq. 2.3 [25]:

Another more general form can be derived when combining Bruggeman with Polder

and van Santen approach. This form is known as the extended Bruggeman (EB) and is a function

of the depolarization factor N, which is a geometrical factor that accounts for the geometry of the

inclusions. The general form of the EB model is given by Eq. 2.4 [26, 27],

All of these models are used to describe the effective dielectric properties of mixtures in

the THz range but with certain conditions. For example, Maxwell-Gamett theory calculates the

effective dielectric properties of a material formed by the presence of small (spherical) particles

embedded in a host material [24], The Bruggeman model is used to calculate the effective

Eq. 2.3

f - 1 _ (Eh\i 3N+1 J ( e p ~s k \ (h ~ U J U-e J V'

( l+3N)Ep + ( S - 3 N ) £ h \ [ 9N2-12N-5(l+3N)£p+(5-3N )£R

[—3N2 + 3/V] 12/V— 18N2— 2 9W2 —12JV—5

Eq. 2.4

15

dielectric properties of many components in a mixture [25]. For this reason, it is important to try

several effective medium models and then choose the model which best fits the experimental

data [25]. In this work, a new model that incorporates a Bruggeman EMT model combined with

a Maxwell-Garnet EMT (MG-EMT) is described, and shown to be effective for extracting

density and MC from THz measurements for the wet wood. Due to the random distribution of

water molecules in the wet wood, a Bruggeman EMT model was used to obtain an effective

medium approximation for the hydrated cell wall, while MG EMT model was used to obtain an

effective medium approximation for the oven dried cell wall because it can be modified to

account for the cylindrical symmetry of the wood system.

As mentioned above, the appropriate effective medium model depends strongly on the

internal structure of wood. Wood structure varies between species and in order to use the best

EMT model, information about the wood structure should be examined in more details.

2.6 Wood structure

Simply, wood is a natural and renewable material, which is widely used in construction,

and more and more engineered wood products are continually being developed. Chemically,

wood is a porous material consisting mainly of cellulose, hemicelluloses and lignin.

Anatomically, the structure of wood is complicated, but in simple terms, the cell wall of wood is

a repetitive array of cylindrical pores.

Wood species are classified into two groups: hardwoods and softwoods. Hardwood and

softwood trees are botanically different. They are included in the botanical division

16

spermatophytes, which mean that they produce seeds. Softwoods are in the gymnospermae

subdivision and hardwoods are in the angiospermae subdivision [28]. Softwood trees are

characterized by needle-like leaves in contrast to hardwood trees which are leaf-bearing. [28].

As shown in Fig. 2.6 and Fig. 2.7, the wood of a hardwood tree is much different than

that of a softwood tree. Hardwoods are composed of different types of cells and have more

complex anatomical elements in contrast to softwoods which usually have a uniform

arrangement with fewer complex cell types. Hardwoods are also normally denser than

softwoods. These factors mean that hardwoods will interact in a different way with THz

radiation than softwoods. Due to the difference in structure between hardwoods and softwoods, it

is necessary to consider both types of species in order to determine how density changes

according to their internal structure. The structure of each wood species will be introduced in

more details in the next section.

2.6.1 Softwoods and Hardwoods

The main difference between softwoods and hardwoods is found in the microscopic

structure of wood. Softwood contains two main types of cells: longitudinal wood cells (called

tracheids) and transverse ray cells (called parenchyma). The tracheids are responsible for the

mechanical support and the water conduction functions in the tree. The parenchyma cells are

responsible for nutrients storage. Hardwoods have fiber cells for support and vessel elements for

water conduction. The softwood tracheids are about four times longer (approximately 2.5-5

millimeters) and ten times narrower than hardwood vessels. The difference in internal structure

of softwoods and hardwoods can be clearly seen in Fig. 2.6 and Fig. 2.7. Another difference

between softwoods and hardwoods is that softwood tracheids are closed at each end with tiny

17

openings called pits, as shown in Fig. 2.8, while hardwood tracheids are open at each end and are

free of pits.

Resin canal

Parenchyma

Eartywood tracheids

Latewood tracheids

Ray cells

Fig. 2.6 Softwoods internal structure [30].

18

Fig. 2.7 Hardwoods internal structure [30],

19

cytoplasm absent (cells dead at maturity

companion cM (living)

tracheids conducts water and Conducting cells are dead dissolved minerals and hollow at maturity

F ig . 2.8 Softwood (left) and Hardwood (middle, right) cell wall structure [28],

Since there are different anatomical structures between hardwoods and softwoods, the

density is different. This means that their reaction to any variation in the environmental

conditions (temperature and humidity) will cause changes in moisture content. For this reason,

different wood species from hardwoods and softwoods will be chosen in this work to investigate

how their densities change with changing moisture content and if the internal structure has an

effect.

2 0

2.7 Moisture content

Wood is a hygroscopic material where the MC will change based on the surrounding

relative humidity (RH) and temperature (T). Wood swells or shrinks depending on the increase

or decrease in its MC. When wood is exposed to constant temperature and humidity, it achieves

equilibrium moisture content (EMC). Moisture content in this study is defined as the percentage

difference between the wet mass and the oven dried mass:

EMC = (E lin h A x 100% , Eq. 2.5V mod J

where m is the wet mass and m od is the oven-dry mass [37, 38].

Chemically, wood is composed of hemicelluloses, cellulose, lignin and water. Water in

wood is found in two different forms, free water (liquid-like) and bound water. Free water is

contained in the cell lumen voids and is held by capillary forces only. Bound water is chemically

bound to the cell wall by intermolecular hydrogen bonds with the hydroxyl groups of the

cellulose molecule. Fig. 2.9 shows how the two different kinds of water found inside the wood

material. When the cell walls are saturated with bound water without any free water found in the

cell lumens, the wood is referred to being at the fiber saturation point (FSP).

2 1

Fig. 2.9 Free water and bound water inside wood [31].

The presence of bound water in wood softens the cell walls and the hydrogen bonds

between cellulose and water are stronger than between cellulose, making hydrogen bonding with

water energetically more favourable. Therefore, the cellulose microfibrils are no longer strongly

bonded to each other, making it easier to move leading to a decrease in the stiffness of wood

[32].

2.8 Density

Wood density is considered an important wood quality attribute. There are several

definitions of density including basic density, defined as the weight of oven dry wood at

22

maximum volume (MC > fibre saturation point) [33]. Generally, density is measured as mass

per unit volume [34]:

where p is the density, m is the mass and V is the volume.

The density of wood is not a fixed value but varies with MC and its mass also changes because

the wood swells or shrinks depending on adsorption or desorption. It also varies from species to

species. For this reason, the ability to simultaneously predict density and MC is important for the

wood industry. To do this, a non-destructive wood inspection tool is highly desirable.

2.9 Applications of THz technology

THz radiation has been studied for a wide range of applications, including applications

in security [3], the spectroscopy of pharmaceuticals and explosives [3], medical applications [4]

and quality control [14],

Applications of THz radiation are seeing significant interest at the present time. There

are many potential uses in the wood products industry for process quality control based on wood

properties such as density, grain angles and moisture content. It was determined early on that

THz radiation could be used to create a density map of beech wood with sub-annular ring spatial

resolution [5]. The prediction of wood density in that work was based on a strong relationship

between the absorption coefficient of the wood and the density at THz frequencies [24],

23

Further studies have recently shown that predicting the oven-dried density of wood

using THz-TDS is possible [35], The results showed a very good correlation over 46 wood

species, indicating that THz spectroscopy is applicable to a wide range of very different species.

An effective medium theory (EMT) was applied to predict the density from the THz

measurements. The Maxwell Garnet (MG) model discussed in section 2.6 was modified for a

cylindrical symmetry, and used to describe the THz-wood interaction. This model was based on

analyzing the effective polarizability of cylindrical inclusions and was shown to work very well

for the case of oven-dried wood [35]:

= f £az£cw , Eq 2 7£ e f f "t" £ c w e a + £ c w

where seff is the effective dielectric constant of the cell wall material; ecw is the dielectric

constant of the cell wall material; ea is the dielectric constant of air (assumed to be 1); and fa is

the volume fraction of air.

The properties of wood change with changing moisture content and another model

capable of incorporating large dielectric contrasts (for including water) is needed when

measuring the dielectric constant of the wet cell wall material. Wood naturally contains some

moisture, which has an impact on the strength, stiffness, or durability of wood products. The

simultaneous measurement of density, gross fiber structure and moisture content makes THz

technology an interesting tool for the wood products industry.

24

2.9.1 Using terahertz radiation to probe wood

THz Measurement configurations

The experimental configuration of a THz-TDS system is usually either in transmission

or reflection. A Transmission geometry is highly desirable for applications, and is the geometry

used in this work and is discussed in more details in the next sections.

Transmission

In this configuration, the emitter and detector were arranged in a line. A sample holder

on a rotation mount was placed in between the transmitter and detector to hold the sample. The

sample can be mounted at any angle using this holder. Usually, an aperture or lens is used to

narrow the beam so the beam passed only through the sample.

The measurement procedure for the transmission geometry was as follows: (1) a

reference scan was taken with no sample is place, (2) a background scan was taken by blocking

the holder using a material that is opaque to THz radiation, (3) a scan of the sample was taken to

compare to the reference using certain models that will be discussed later. The transmission

configuration setup was as shown in Fig. 2.10.

25

Fig. 2.10 THz transmission spectroscopy.

2.9.2 Analysis of THz Data

In this section, the methods of extracting the information from the collected data are

discussed in more details.

Phase unwrapping

Phase information is required to calculate the index of refraction and absorption

coefficient from the collected THz data. According to Duvillaret et al., the measured signal is

very small compared to the noise level at low frequencies [38], which results in a phase that may

not go to zero at zero frequency as must physically happen. The distorted phase at the low

frequency points is linearly extrapolated [39] to account for this, and implemented in the analysis

conducted in the experiments that follow.

Data is collected using transmission geometry. To analyze the data, the Matlab

programming language was used to solve for the index of refraction and the absorption

coefficient. Two different methods were used to analyze the data: (1) the thick sample

approximation of Duvillaret [39], and a purely numerical scheme (the inverse problem) (2) [40].

26

The complex dielectric function is calculated from the THz measurements by using the

thick-sample approximation of Duvillaret [40]:

E w o o d ( v ) £ £— T~r~ lA W l WA Eref\v)

exp | _ l2 E ± _ ^ a ) ] j Eq 2.8

where Eref ( v ) is the electric field amplitude of the reference spectrum, Ewood(v) is the electric

field amplitude of the transmitted spectrum, v is the frequency, L is the thickness of the wood

sample under study, c is the speed of light, nw is the refractive index of wood, na is the

refractive index of air, tAW and tWA are the Fresnel transmission coefficients from air to wood

and wood to air respectively which can be found for normal incidence as given by:

2ili C T OEq. 2.9V fii+nj ’

where n* is the index of refraction for the first material, n;- is the index of refraction for the

second material. In our case, the two indices will be those of air and wood. The index of air is

taken to be 1 and the index of wood is a complex value defined as:

n w = 7lw + ikw , Eq. 2.10

where nw and kw are the real and complex index of refraction for wood respectively.

The index of refraction and absorption coefficient of wood is calculated as [36]:

OCn w = ----------+ 1 , Eq. 2.11

w 2nvL H

21

where ocw= Anvkw/c, R and 6 are the amplitude and phase of the ratio of the reference field to

the transmitted field when written in Euler form,

- tranf f = R e W, Eq. 2.13E re fiv ) ’ 4

where £re/(v ) is the reference field in the frequency domain, and Etrans (v) is the transmitted

field in the frequency domain.

2.9.3 The inverse electromagnetic problem

The refractive index can also be measured by measuring the effect caused on the electric

field of a THz wave after passing through the material under study as presented in [40].

Assuming E**f (o i) and Etrans (co) are the measured reference and sample signals, the frequency

dependent transfer function can be written as [40]:

Hexperlmm, M = , Eq. 2,14

28

Air(0)

binit Po V l ^ o

Emit?0T01PiT10R210

Fig. 2.11 Fabry-Perot reflections.

As shown in Fig. 2.11, the signal propagation through the sample is divided into several

stages. First, the incident signal Einit on the front (left) surface of the sample split into two

signals, reflected and transmitted [40]. The reflected signal is not a part of Efrans and so will be

discarded. The transmitted signal is equal to Einitt01 and propagates through the sample [40],

This transmitted signal has an electric field of Einitt01Pfll) on second (right) surface of the

sample. At this surface, the signal splits again into reflected and transmitted signals [40]. The

transmitted portion has an electric field of Einittoi^iCO^io anc* is a part of Etrans. This leads to

the well-known Fabry-Perot reflections [40]. The THz pulse propagates through air between the

two antennas, which is taken into account by the propagation factor P0. After collecting all of the

multiple reflections, the overall field can be written as [40]:

^trans ~ EinitPa(.x ~ 0^01?l(0^1o[l + £f=l(r10̂ 1 ) '] ’ Eq. 2.15

E,init

Sample

29

where 5 represents the number of Fabry-Perot reflections, I is the thickness of the sample, r01 is

the Fresnel reflection coefficient from air to sample, and t01 is the Fresnel transmission

coefficient from air to sample, which can be calculated using Eq. 2.9. The reference THz field

propagates through air only, and is calculated by [40]:

E ref = EinitP0(x), Eq. 2.16

Now, the theoretical transfer function can be written as [40]:

= i g f = '>o(-Oto./Vio[l + Zf-iWoP,2)1], Eq. 2.17

The material parameters n and k can be extracted numerically from this transfer function. To do

this, a range of values for n and k are assumed, and the values are varied until Htheo is arbitrarily

close to Hexp. In order to achieve proper convergence, the number of Fabry-Perot reflections

must be assumed. This can be done by assuming an initial value for n and k as follows [40]:

Etrans.max ~ Ere f ,m a x -^ P ( Co ^1^)' ^T 2.18

where Etrans max and Eref max represent the maximum field of the transmitted and reference

signals respectively.

k1 = - 1 fa logfegaggsl, Eq. 2.19l (i) pre/.m aiI

At = — , Eq. 2.20Co

n i = ^ + n0, Eq. 2.21

3 0

where At is the time delay between the two signals, 1 is the sample thickness, c0 is the speed of

light, and An is the index difference between wood and air.

Assuming tmax is the maximum time of a measurement since the incidence of the reference

signal, which is taken to be the temporal window of data collection. The THz beam propagates

along a path of length equal to the sample thickness I with a speed — inside the sample. So, theni

number of Fabry-Perot reflections 8 is the greatest integer that satisfies the following relation

[40]:

W ^ - K l + 2

Chapter 31

Simultaneous prediction of density and moisture content of wood by terahertz time domain spectroscopy

3.1 Abstract

In this study, demonstration of simultaneous prediction of solid wood density and

moisture content, both of which are critical in manufacturing operations, of 4 species (Aspen,

Birch, Hemlock and Maple) was accomplished using terahertz time-domain spectroscopy (THz-

TDS). THz measurements of wood at various moisture contents were taken for two orientations

of the THz field (parallel and perpendicular) with respect to the visible grain. The real and

imaginary parts of the dielectric function averaged over the frequency range of 0.1 to 0.2 THz

strongly correlate Awith density and moisture content of the wood. We extend a model

1. T. Inagaki, B. Ahmed, I. D. Hartley, S. Tsuchikawa, and M. Reid, " Simultaneous prediction o f density and moisture content o f wood by terahertz time domain spectroscopy", J Infrared, Millimeter, and Terahertz Waves. (2014) 35:949-961.

32

previously applied to oven-dry wood to include the effects of moisture below the fiber saturation

point by combining two effective medium models, which allows the dielectric function of water,

air and oven-dry cell wall material to be modeled to give an effective dielectric function for the

wood. A strong correlation between measured and predicted values for density and moisture

content were observed.

3.2 Introduction

Wood is a natural material widely used for its versatility and strength in construction.

There are significant variations in the properties of wood (density, moisture content and grain

angle for example) within and between species, which affect structural properties, and therefore

dictate performance characteristics. When wood is processed industrially, where uniformity of

the raw materials is critical for the reliability of the end product, such variations in physical

properties must be measured at least, and preferably controlled.

There is a strong relationship between the density of wood and its moisture content,

namely, as moisture content increases, density increases. Further, an end-use product such a

dimension lumber must have certain strength to meet grading rules criteria for market consumers

[41]. To meet the rules, the lumber is tested for its modulus of elasticity, which is based on

density [42], As well as the impact of density, the grading rules also dictate that the moisture

content be within a specific range. Measuring both density and moisture content has been done in

a laboratory setting, but not on an industrial scale.

33

The wood cell wall consists of cellulose, hemicellulose, lignin and extractives. The

density of cell wall is almost the same for all species of wood (about 1.4 g cm-3) [43]. However,

since the size of the cell and cell wall thickness (the ratio of the cell wall to air) differ between

species, the density of wood varies from about 0.1 to 1.2 g cm-3.

Given the above, wood density strongly influences such properties as the modulus of

elasticity (MOE) and stiffness, which play a critical role in the manufacturing of wood products.

Generally, higher density wood has a higher MOE [42]. Determining the MOE of wood can be

done using non-destructive methods such as static bending [42], stress-wave propagation [44],

microwave [45] and near infrared [46] with an overall goal of using such techniques for in-line

applications.

The dry basis moisture content (MC) of wood is defined as the ratio of water mass in

wood to the mass of oven-dry wood. In a living tree, there is free water, which exists in the

lumen or free space in the wood, and bound water, which is held in the amorphous region within

the cellulose, hemicellulose and on the surface crystalline region of cellulose by hydrogen

bonding [32], When the wood is dried, free water is preferentially evaporated into the

atmosphere. Around a MC of 25-30 %, which is known as the fiber saturation point (FSP), all

free water is evaporated. The bound water strongly affects the properties of wood, and so control

and monitoring of MC during the manufacturing process is important [33].

Terahertz (THz) radiation has the potential to be a useful tool for sensing and imaging

of wood because wood is relatively transparent at these frequencies (below about 1 THz), the

wavelengths are sub-mm which offers good spatial resolution for imaging, and THz radiation can

probe the gross fiber structure of wood. There have been several reports on the interaction of

34

THz radiation with wood [5, 14, 38, 48-51], which have highlighted applications of THz

radiation to the wood products industry, including density mapping [5], defect detection [14],

properties of paper [52] and wood-plastic composites [53], dendrochronology [6], and sensitivity

to internal moisture suitable for imaging of MC [51].

To date, the prediction accuracy of various species of wood by THz spectroscopy has

been demonstrated on oven-dried wood [38], and requires quantification over a range of moisture

contents in order to further our understanding of THz-wood interactions so that new applications

of this emerging technology related to wood science and the wood industry can be explored

further. We showed an excellent correlation between the predicted and measured volume

fractions of cell wall material (density) over a large range of volume fractions (f= 0 .2-0 .8), by

applying a Maxwell Garnett (MG) effective medium theory (EMT) approach [38], Here, we

show the prediction accuracy is retained over a range of moisture contents below the fiber

saturation point, and also demonstrate the possibility for simultaneous extraction of MC and

density.

3.3 Materials and Methods

3.3.1 Sample preparation

Aspen (Populus tremuloides, Povenw ood~ 0.49 g cm-3), birch (Betula spp, Povenw ood ~

0.64 g cm-3), Western hemlock (Tsuga heterophylla, Povenwood~0-36 g cm-3), and maple (Acer

saccharum, Povenw ood~ 0.72 g cm-3) woods were obtained from a local supplier. Povenw ood is

the density of oven-dry wood. Three groups of 5 samples for each species were prepared. The

35

samples were cut from the radial plane into wafers roughly 5 mm thick and 30 x 30 mm square,

and the surfaces were sanded lightly to a smooth finish.

At first, the samples were dried in a convection oven for 48 hr at 103±2 °C to determine

the oven-dry mass. Before and after the THz measurements, the samples were weighed (±0.01 g)

in order to be certain that the samples did not absorb water from the atmosphere. The dimensions

(length, width and thickness) of the samples were measured using digital calipers (±0.01 mm)

before all THz measurements. After the measurement of oven-dry wood, the samples were

conditioned at different relative humidities (RHs) to obtain different MCs. This was done in a

step-wise approach using desiccators where the RH was controlled with saturated salt solutions.

The salts used were: anhydrous calcium sulfate (CaS04 , RH = 0%), potassium hydroxide (KOH,

RH = 8%), potassium fluoride (KF, RH = 30%), sodium dichromate (Na2Cr2C>7-2H2C), RH =

54%), ammonium chloride (NH4CI, RH = 77%) and potassium nitrate (KNO3, RH = 94%)

obtained from SIGMA-ALDRICH. A desiccator with water only was used for obtaining 99%

RH. The samples were left for at least 48 hrs in the desiccators to ensure that they reached an

equilibrium MC. After equilibrium was reached in the first step (RH = 11%), determined by no

change in mass, the samples were removed and their mass and dimensions were recorded. THz

measurements were taken immediately for two orientations of the THz field (parallel and

perpendicular) with respect to the visible grain. The sample masses were recorded after THz

measurements to ensure that the samples did not absorb or desorb water. After the THz

measurements, the samples were placed in the next higher RH (that is, RH = 32%). Densities and

MC were calculated from the physical dimensions and the averaged mass of the samples and

mass of the oven-dry wood samples. This process was repeated for each MC progressing from

3 6

low to high MC. The experiments and wood conditioning were conducted at room temperature

(21±1 °C).

3.3.2 THz spectral measurement

Polarized THz transmission spectroscopy was performed using a modified Picometrix

T-Ray 4000 THz spectrometer. This system produces THz measurements in an 80 ps window at

a rate of 1000 waveforms per second. The bandwidth extends from approximately 0.01-2.00

THz. For each species of wood studied, the time-domain waveforms of the transmitted terahertz

radiation were recorded at 0° and 90° orientation of the grain with respect to the terahertz

polarization, each measurement being an average of 10,000 waveforms. A reference THz signal

without a wood sample in place was obtained prior to each transmission measurement. The

sample sizes are chosen to be larger than the THz beam diameter to avoid diffraction effects. The

THz spectroscopy was performed in transmission, with a THz beam diameter (1/e electric field)

of approximately 30 mm. The complex refractive index of the samples was determined from a

transmitted and reference THz pulse according to [39] in the thick sample approximation as

outlined in [46], The complex refractive index was used to calculate the dielectric function in

order to apply the effective medium theories (EMTs) described in this work.

3.4 Results and discussion

Relation between dielectric function and oven-dry density and MC

37

Fig. 3.1 shows the moisture content change with relative humidity. Bound water exists

in wood below the FSP, and behaves differently than free water as it is chemically bound by

hydrogen bonding in the amorphous regions of the cellulose, hemicellulose and on the surface

crystalline region of cellulose. Because the distribution of the chemical components does not

vary greatly between species of wood, it is not expected that there are large differences in

sorption behavior, which is reflected in Fig. 3.1.

c9

23m*os

25

20

15

10

5

060 1000 20 40 80

Relative humidity (%)

Fig. 3.1 Dependence of moisture content (oven-dry basis) on the variation in relative humidity

for maple (open circle), aspen (filled circle), birch (open square) and Western hemlock (filled

square).

Fig. 3.2 shows the measured frequency-resolved (a) real part and (b) imaginary part of

the dielectric function, e , obtained from THz transmission spectroscopy of oven-dry wood. Plots

(c) and (d) show the real and imaginary parts of the dielectric function averaged over the

38

frequency range of 0.1 to 0.2 THz, respectively. The THz beam is polarized perpendicular to the

visible grain. A strong correlation between oven-dry density ands is observed consistent with

other research [5, 14, 38, 55, 56]. The spectral range from 0.1 to 0.2 THz was used in this study

in order to remain approximately in the wavelength range of validity for MG-EMT. As shown in

Fig. 3.3, the real and imaginary part of s show a strong correlation with moisture content. These

strong correlations between the real and imaginary part of e and oven-dry density and moisture

content suggest the possibility of simultaneous prediction of both quantities from the measured

THz signal.

!w'o«aT6©cc

I01a

2.4

2.2

• Maple2 Maple

Birch

1.6 •AspenAspen

• Hemlock1.4 Hemlock

1.2

1

0 1BirchAspenHemlock

0.08Maple

0.06Birch

Aspen0,04

0.02

00 0 1 0 2 0.3 0 4 0 5 0.3

Frequency (THz)0.4 0.5 0.6 0 7

Oven dry density (g cm 3)08

Fig. 3.2 Frequency-resolved (a) real part and (b) imaginary part of the dielectric function

obtained from THz transmission spectroscopy of oven-dry wood. Relation between oven-dry

density and (c) real part and (d) imaginary part of dielectric function averaged over the frequency

39

range of 0.1 to 0.2 THz (polarization of the THz field is perpendicular to the grain of the wood

samples).

?LLhio«a.

y * 0.0196x^1.8685

?ILr o-4'o| 0.3O.

.6 0-2 9tsE

y = 0 0004*' * O.OOSx + 0 0568

0 0.1 0 2 0.3 0 4 0 5 0 5 10 15 20 25Frequency (THz) Moisture content (%)

Fig. 3.3 Frequency-resolved (a) real part and (b) imaginary part of the dielectric function

obtained in transmission spectroscopy of Birch at various moisture content. Relation between

moisture content and (c) real part and (d) imaginary part of dielectric function averaged over the

frequency range of 0.1 to 0.2 THz (polarization of THz field is perpendicular to grain of wood).

In order to extract a measurement of the density and moisture content from the THz

measurement, a model is required that describes the dependence of the dielectric function on

them. Next, a model is described that incorporates a Bruggeman EMT model combined with a

4 0

Maxwell-Garnet EMT (MG-EMT), and shown to be effective for extracting density and MC

from THz measurements.

Simultaneous prediction of density and moisture content of wood species from THz

measurements

A self consistent scheme (SCS) approximation of the elastic properties of materials

[54], easily generalized to optical properties [57, 58], which specifically relates to a cylindrical

geometry has been proposed by Hashin and termed the composite cylinder assemblage (CCA)

scheme [54]. In this model, the effective medium properties are derived by inserting an infinite

cylinder with dielectric function Ej in a concentric cylindrical shell of dielectric function e2,

having radii a and p, respectively, as shown in Fig. 3.4, and solving the boundary problem for the

effective dielectric function (eeff) of the material.

4 1

Fig. 3.4 Composite Cylinder Assemblage (CCA) scheme where a cylindrical inclusion of

dielectric constant is ej surrounded by a cylindrical shell of dielectric constant s2 leading to a

bulk effective dielectric function £eff.

In order for this calculation to be possible, the ratio of must be specified. Hashin has

shown that by assuming this ratio is the volume fraction of particulate phase (of dielectric

function Ej), and therefore the concentric cylinders retain the volume fractions of the entire

composite material, that a best possible upper bound on the effective dielectric function is given

by (for the case where the field is polarized perpendicular to the axis of the cylinders):

±,max _ , h t i£eff — e2 + l | f2 > E q . 3 .1

E J-C 2 2e2

42

Where £jcorresponds to properties of the core phase, and e2 corresponds to the properties of the

matrix (shell) phase. This also happens to correspond to the MG formula used for analyzing

cylindrical systems [5, 58]. The MG formula for infinite cylinders when the field is polarized

perpendicular to the axis of cylindrical symmetry is usually written as:

SsilS = f Eq. 3.2

In this study, it is of interest to extend the model used previously for density of oven-dry

wood [38] to include the effects of moisture, in particular, below the FSP. In this context, the

geometry retains a cylindrical symmetry, and the MG-EMT (upper bound of the CCA) will be

used to reflect this. However, the dielectric function of the cell wall material does change with

moisture content as a result of the adsorption of bound water. Since the distribution of water in

the cell wall is expected to be random (non-geometrical in nature), a Bruggeman EMT model to

obtain an effective medium approximation for the hydrated cell wall seems appropriate. Indeed,

an EMT was proposed to handle the incorporation of water within paper, which is a cellulose

fiber network [52], and worked extremely well for predicting moisture content. The same

approach is adopted here to handle the moisture within the cell wall material. The Bruggeman

EMT is given by:

£eff = 4 + Jp2 + 8e1£2̂ , Eq. 3.5

p = (3fj - 1 )si + (3f2 - l)e2, Eq. 3.6

In order for this to work, the dielectric properties of both the cell wall material, and the

water in the cell wall must be known. It was found previously that a single (complex) value for

the cell wall material could be assumed, allowing density prediction over 40 species of wood

[38]. We adopt that value here (as discussed below). For the water, we use the well-known

double Debye model appropriate for frequencies around 1 THz [59]:

e((0) = i Jl£L + i lZ ^ + £ccj Eq. 3.71 —-ICOT | 1 -H D T 2

Where the parameters for Eq. 3.7 were taken as presented in Ref. [59]: es = 73.36, £/ = 5.16,t/ =

7.89 ps, £oo= 3.49, and x2 = 0.181 ps.

4 4

The overall model can be described as follows (refer to Fig. 3.5). The dielectric function

of the wet cell wall material is calculated using the Bruggeman model (Eq. 3.5 and 3.6) to

combine the cell wall material and water, which combine in a non-geometric fashion. The wet

cell wall material then makes up the host for a cylindrical symmetry similar to what is seen in

Fig. 3.4. Therefore a MG-EMT with cylindrical symmetry is applied (Eq. 3.2), and the effective

dielectric constant of the wood is obtained by combining the dielectric constant of air and wet

cell wall material using the MG-EMT.

45

wetwood

wetcw

ovencw

Fig. 3.5 Effective medium theory applied to determine the bulk effective dielectric function of

wood at different moisture contents. The dry cell wall material with dielectric constant eovencw

(which is known from measurement - see text for details) is combined with a random

distribution of water assumed to have a dielectric function ewater (see text for details) using the

Bruggeman model to determine the effective dielectric constant of the wet cell wall material. The

MG model with cylindrical symmetry is then applied to combine air, with a dielectric

function eair, and the wet cell wall material to determine the effective dielectric constant of the

W O O d , £vvetwood-

In the first step of computing the dielectric function of the cell wall material, the

geometry is unimportant, and so nothing changes with the polarization of the THz field. In

contrast to this, the step of computing the effective dielectric function of the wood from the wet

cell wall material and air is polarization-dependent. When the THz field is polarized

4 6

perpendicular to the grain, the MG step requires use of Eq. 3.1, whereas when the field is

polarized parallel to the axis of cylindrical symmetry, Eq. 3.4 is used.

This model can be used to simultaneously measure the density and moisture content (by

obtaining the volume fractions f a and fw) of wood samples as follows. A matrix of volume

fractions fa x fw is formed over the region of interest (fa : from 0.3 to 0.8 with 0.005 steps, fw:

from 0 to 0.3 with 0.005 steps). The dielectric function of the wood is evaluated using the EMT

described above, giving eeff for each combination of f a and fw. The availability of a reference

scan then allows the prediction of the transmitted THz waveform as follows. Defining the

Fresnel transmission coefficients from incident material i, to transmitted material t:

t„ = • £ . Eq. 3.8n , + n ,

where n is the index of refraction, and t it is the Fresnel transmission coefficient at normal

incidence. The complex, frequency-dependent transmission function (T(f)) can then be

represented in terms of the complex index of refraction of the wood (nwood = y/£eff)> calculated

from eejf, and given by :

T w oodC O = tavvtwae'2;tfd(fi»00d“ I) , Eq. 3.9

where / is the frequency, and d is the thickness of the wood sample. The effect of the wood

sample on the reference in the frequency domain is given by:

E\vood (0 = T\yood (f)Eref(f), Eq. 3.10

And thus, the predicted THz waveform in the time-domain is calculated by inverse Fourier

transformation:

4 7

E S , ( t ) = C E „ 00(l(f)e-'M dt, Eq. 3.11

We then define a measure of error in the predicted waveform in terms of the sum of squared

difference from the measured waveform:

Err = Si (E^dCt) - C W ) ’ . Eq. 3.12

The only free parameters in the model are the volume fractions of air and water, and the value of

the dielectric function of the cell wall material and water. As discussed above, the dielectric

function of water is taken from ref [60] and is held fixed.

The dielectric function of the dry cell wall material is obtained from the measured

values of permittivity of oven-dry aspen, birch, hemlock and maple. The indices of refraction

and absorption coefficients were determined and averaged over the frequency range of 0.1 to 0.2

THz. The complex dielectric function (e = n2) was calculated from the THz measurements(n =

n + ik). By applying equations (3.2) or (3.4) for the different polarization orientations, the

dielectric function of the oven-dry cell wall material was inferred. The calculated dielectric

functions of the cell wall material of the 4 species of wood were averaged over the frequency

range of 0.1 - 0.2 THz. For the case when the THz field is polarized parallel to the visible grain,

the average of £ovencw over 4 species was 3.36+0.18i, while £0vencwwas 3.39+0.19i when the

THz field is polarized perpendicular to the visible grain. We took the dielectric function of the

dry cell wall as these frequency-independent values.

Reference and transmitted THz waveforms transmitted through samples of aspen wood,

whose density is 0.50 g cm~3 and MC = 2.07%, measured with the THz field polarized

perpendicular to the visible grain is shown in Fig. 6 . Predicted THz waveform gave minimum

4 8

error in terms of the sum of squared difference from the measured waveform when the value of f a

= 0.635 and f w = 0.01 were used. The predicted THz waveform is also shown in Fig. 3.6. The

volume fractions f a and f w obtained were converted to density using the formula,

Pwetwood = Pair X *a + P 0vencw X Povencw + P w X fw* Eq. 3.13

where, fovencw is the volume fraction of the oven-dry cell wall material (fovencw = 1 - (fa + fw)),

Pwetwood *s density of wet wood, povencw is the average density of the oven-dry cell wall

material, which is assumed to be 1.4 g cm" 3 [42], pw is the density of water which is take to be 1

g cm"3, and pajr is the density of air which is taken to be 0.0012 g cm-3at 20 °C.

Moisture contents were calculated using the formula,

Povenwood = Pair X ^ ^w ) + Povencw X ^ovencw- Eq. 3.14

MC = (P- - — sa!lw°°d) x 100 (%), Eq. 3.15Povenwood

where, povenwood is density of oven-dry wood, MC is moisture content of wood. The predicted

values that minimized the error function (Eq. 3.12) for the waveform of Fig. 3.6 gave f a and f„

corresponding to a MC = 2.01% and pwetwood = 0.51 g cm"3.

49

0.7

0.5

0.3

2 0.1

value and n is the number of samples.

Fig. 3.8 shows the relationship between the measured and predicted MC. For both

polarization configurations, the MC was consistently underestimated at low MC, and approached

correct value at high MC. This can be understood based on the behavior of the dielectric function

for water as the amount of bound water increases to approach the FSP. In particular, free water

absorbs much more strongly than bound water, and so at low moisture contents, the use of the

highly attenuating free water dielectric function will result in systematic under estimation of the

MC. In contrast, as the amount of free water increases, the estimation will tend to get better and

closer to the real value as the fraction of total water that is free increases. Furthermore, as shown

in Fig. 3.3, the real part of dielectric function linearly increases with MC, whereas the imaginary

part shows a quadratic increase. This implies that the imaginary part of the dielectric function for

bound water is indeed a function of MC. The stronger absorption at THz frequencies of free

water in comparison to bound water has been described in detail for hydrated lipid systems [61],

and was also directly observed in wood composite systems [53] for MCs below the FSP. In order

to incorporate the MC dependence of the dielectric function of water into our model, it would be

necessary to know the dependence in detail. Since this information is not known at present, it is

beyond the scope of the work presented here.

The main results presented here (Fig. 7 and 8) demonstrate that THz-TDS can be used

for non destructive and accurate measurements of wet wood density over a range of MCs for the

wood species studied here. In addition, the correlation between predicted and measured MCs

indicates that simultaneous MC measurement is possible. In order to accurately predict MC

without a calibration procedure of some type, however, a more detailed model of the dielectric

function of water as a function of MC is required. It should be noted that this behavior could be

51

expected to be species-dependent, at least in part because of the different surface areas exposed

to air in each species (i.e. different porosities). Using both the real part and the imaginary part of

the measured complex dielectric function therefore provides the possibility of simultaneous

measurement of density and MC when the sampling area covers several annual growth rings.

3 0 .7>±t»© 0.6 TJ ■o ©■§ 0.5 t5 ££ 0.4

0.3

(a) Perpendicular

r2 = 0.98y = 1.0152x-0.0038

RMSE = 0.020 g crrf

(b) Parallel

Ay = 0.9925x-0.014 r2 = 0.96RMSE = 0.030 gem '3

0.3 0.4 0.5 0.6 0.7 Q.iMeasured density (g cm-3)

0.3 0.4 0.5 0 6 0,7 0.8 0.(Measured density (g cm-3)

Fig. 3.7 Relationship between measured and predicted density based on MG-EMT model, r 2,

determination coefficient; RMSE, root mean square error, (a) Perpendicular and (b) parallel refer

to the polarization of the THz field with respect to the grain of the wood samples.

52

35(a) Perpendicular

!* • •

(b) Parallel

y = 0.91x-0.8099 ^ = 0.79 RMSE = 3.14%

0 5 10 15 20 25 30Measured moisture content (%)

0 5 10 1510 15 20 25 30 35Measured moisture content (%)

Fig. 3.8 Relationship between measured and predicted moisture content based on MG-EMT

model, r 2, determination coefficient; RMSE, root mean square error. Perpendicular and parallel

refer to the polarization of the THz field with respect to the grain of the wood samples.

Several different EMT models have been used to study properties of composite

materials at terahertz frequencies [62], It is somewhat commonplace in the THz literature to

choose an EMT that best fits the experimental data [63]. Therefore, it is appropriate to review

different EMT models in relation to what has been used here.

A comprehensive review of different EMT models that have been used for THz

applications has been published previously [62], The geometry-independent models suitable for

use as the mixing rule for the wet cell wall material (water + cell wall material) are the

Bruggeman model, and the Landau, Lifshitz, Looyenga (LLL) model [62], While the latter can

be used for mixtures with large dielectric contrast [53], the former model has been applied here

as it worked exceptionally well for water in paper [52], which is chemically similar to the wood

53

cell wall material. The second component of the model is the geometry-dependent component

suitable for a cylindrical symmetry exhibited by wood structure. When the THz field is polarized

parallel to the visible grain, then the THz field will always lie in the boundary between two

interfaces, and so follow the simple mixing rule given by Eq. 3.4 [58]. That this model gives

good agreement for the density prediction across moisture contents of Fig. 7 is evidence that the

Bruggeman model is appropriate for the cell wall material.

For the polarization of the THz field perpendicular to the axis of cylindrical symmetry,

in addition to the MG-EMT used previously [38], there is the Polder and van Santen (PvS) model

for rod-like shapes, and a modified Bruggeman model appropriate for rods [62] that could be

appropriate for wood related to the work presented here. The PvS and modified Bruggeman

models lead to dielectric functions that lie within the bounds of Eqs. 3.1 and 3.3, and in practice,

we find that the predictive power of the model gets progressively worse with models that move

away from the upper bound and towards the lower bounds described by Eqs. 3.1 and 3.3.

3.5 Conclusion

Moisture content and density of 4 species of wood were simultaneously measured by

means of THz time domain spectroscopy. The real and imaginary parts of the complex dielectric

function have a strong correlation with density and moisture content. A model combining

Bruggeman and MG EMTs was proposed and shown to have good predictive power for density

and MC simultaneously. It was observed that the results for predicting the MC imply that the

dielectric function of water in wood changes as a function of moisture content as the water goes

from bound at low MC to free at high MC, consistent with other reports. In order to predict MC

54

beyond correlations, it was determined that more work is required to understand the MC

dependence of the dielectric function of water in wet wood. The ability to simultaneously

measure density and MC over a range of MCs below the fiber saturation point make THz

radiation an attractive new technology for probing wood properties.

55

Chapter 4

Investigation of the moisture content desorption in wood by terahertz time-domain spectroscopy

4.1 Abstract

Terahertz time-domain spectroscopy was used to investigate the dielectric constant of

water in 4 wood species (Aspen, Birch, Hemlock and Fir) at different moisture contents.

Applying THz-TDS, changes in the absorption coefficient and refractive index of water absorbed

into wood are observed and characterized. An effective medium theory was applied to determine

the effective dielectric function of wood at frequencies between 0.1 and 0.5 THz at different

moisture contents. A model was proposed to describe the dependence of the dielectric function of

water on the varying moisture content.

5 6

4.2 Introduction

Wood is a hygroscopic material whose moisture content (MC) depends on the

surrounding relative humidity (RH) and temperature (T). Wood swells (or shrinks) in response to

increasing (or decreasing) MC. When wood is exposed to a fixed relative humidity at constant

temperature, the wood will develop the same MC as the surrounding atmosphere, which is

known as the equilibrium moisture co